An energetic approach to the wear behaviour of
plasma-sprayed alumina–13% titania coatings
A. Rico, M.A. Garrido, E. Otero, J. Rodrı´guez*
Departamento de Ciencia e Ingenierı´a de Materiales, Universidad Rey Juan Carlos, 28933 Mo´stoles, Madrid, Spain
Received 28 December 2009; received in revised form 29 June 2010; accepted 1 July 2010 Available online 31 July 2010
The wear behaviour of plasma-sprayed Al2O3–13% TiO2coatings was determined by pin-on-disc tests that were performed at diﬀerent
normal loads. Conventional coatings, deposited from micrometric powders, and modiﬁed coatings, deposited using agglomerates of nanoparticles as feeding powders, were studied. The wear rates of conventional and modiﬁed coatings were compared, and the inﬂuence of the microstructure was analysed by using an energetic approach to the wear. The enhanced properties of the modiﬁed coating were justiﬁed in terms of its microstructure. It is likely that the partially melted zones in this coating were responsible for the improvement in the wear resistance via their reinforcement of the ceramic matrix composite.
Ó2010 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved.
Keywords: Ceramic coatings; Plasma spraying; Wear; Nanostructure
Ceramic coatings are used in tribological applications because of their favourable combination of properties: low density, hardness and chemical inertness. Coatings that are based on alumina are a good alternative when wear resis-tance is the limiting factor. However, the main drawback to using alumina-based coatings is their brittleness[1–3]. In order to increase the toughness of a coating, diﬀerent quan-tities of other ceramics can be blended with alumina to main-tain a balanced equilibrium between properties. Titanium oxide has a low melting point and plays a role in binding the alumina grains. Coatings of higher density with suitable hardness and increased toughness can be achieved through the blending of ceramic materials and alumina[4–6].
Alumina–titania coatings are usually manufactured by atmospheric plasma spraying. Under the high temperatures involved, coatings with a good adherence to the substrate and a limited level of porosity can be produced. The
inﬂu-ence of the projection parameters on porosity, hardness, Young’s modulus and wear resistance has been extensively studied in the alumina–titania system[1,6,7].
Following the growing interest in nanomaterials[7–14], modiﬁed plasma-sprayed alumina–titania coatings have also been prepared from nanocrystalline powders. Two main diﬃculties are encountered during the manufacture of the coatings: the small size of the nanoparticles impedes their direct projection in conventional plasma equipment, and the elevated temperatures that are presumably reached in the plasma may destroy the original nanostructure dur-ing thermal spraydur-ing if the process is not carefully con-trolled[7,9].
A new technological process was developed for prepar-ing agglomerates of nanoparticles by spray-dryprepar-ing . The average sizes of the agglomerates are similar to those of conventional powders (approximately 30–50lm). These agglomerates can be projected using standard plasma equipment. The nanostructure can be maintained if the temperature during plasma spraying is held at an interme-diate value between the melting points of alumina and tita-nia[7–14].
1359-6454/$36.00Ó2010 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved. doi:10.1016/j.actamat.2010.07.001
E-mail address:email@example.com(J. Rodrı´guez).
Recently, the mechanical properties and the wear behav-iour of the modiﬁed alumina–13% titania coatings have been studied [16–18]. Although a better wear resistance was reported, these studies did not use a systematic approach toward understanding the wear mechanisms, the variables and the parameters controlling the wear process.
Wear behaviour is not an intrinsic material property due to its dependency on the properties of the materials that are making contact (microstructure, roughness, grain size, mechanical properties) and with the conditions under which tests are performed (contact geometry, normal pres-sure, temperature, sliding velocity). There are many articles on the topic of the wear of ceramics, and several wear mod-els have been proposed that describe the characteristic brit-tle fracture mechanism. The eﬀorts of Evans, Hsu, Ashby, Kato and their colleagues must be recognized[19–36]. Hsu and Shenpointed out that most of these models were developed for speciﬁc pairs of materials under deﬁned operating conditions, and it is diﬃcult to apply these mod-els to other systems.
In this work, a comparison of the tribological behaviour of conventional and modiﬁed alumina–13% titania coat-ings was carried out under diﬀerent normal pressures. Two coatings were produced based on micro-sized and nano-sized feedstock; these coatings had the same compo-sition but diﬀerent microstructural features. We investi-gated the link between the microstructure and the local mechanical properties, the global eﬀective properties and the wear response.
2. Materials and experimental techniques
Al2O3–13% TiO2coatings that were deposited on SAE-1042 steel by atmospheric plasma spray (APS) were studied. Conventional coatings were fabricated from commercial powder (METCO 130 provided by SULTZER METCOe). The average particle diameter was approximately 50lm.
Modiﬁed Al2O3–13% TiO2coatings were prepared from agglomerates that were supplied by INFRAMAT ADVANCED MATERIALSe. The original material was developed by Gell et al.[9–11] and is under a patent by INFRAMAT ADVANCED MATERIALS. The agglomerates were manufactured by spray-drying nano-metric particles (NanoxeS2613S) with an average size of 200 nm. Small additions of ZrO2and CeO2were included in order to improve the ﬂow of the powder in the plasma and to increase the adhesion of the coating. The agglomer-ates, which had an average size of 30lm, can be projected with standard APS equipment.
A Ni–Al–Mo 90/5/5 (wt.%) bond coat was deposited between the substrate and the ceramic coating to improve the adhesion. The ﬁnal thickness of the coating was approx-imately 500lm, including the bond coat. The parameters controlling the APS process are included inTable 1.
2.2. Experimental techniques
2.2.1. Microstructural characterization
To perform a microstructural analysis, several samples were cross-sectioned using a diamond disc and metallo-graphically prepared. The samples were analysed by scanning electron microscopy (SEM) using the Philips XL30 and JEOL 6400 microscopes. The microscopes were equipped for energy dispersive X-ray microanalysis. To determine the morphology and the composition of nanopar-ticles and agglomerates, some samples were prepared for analysis with transmission electron microscopy (TEM) in an FEI Tecnai 20 operating at 200 kV.
2.2.2. Mechanical characterization
Samples were prepared in plan view from the as-sprayed coatings. The samples were cut with a diamond saw and polished using 1200 grit SiC paper. These steps were fol-lowed by a subsequent polishing in a diamond slurry up to a 0.25lm ﬁnish. Time and pressure was carefully con-trolled in order to minimize any artiﬁcial increase in the surface porosity or the excessive removal of poorly bonded regions. Finally, the polished surfaces were cleaned in deionized water, and were then cleaned by ultrasonication in propanol.
Depth-sensing indentation tests were carried out using a diamond Berkovich indenter with a nominal edge radius of 100 nm. The experimental device was a Nanoindenter XP (MTS System Co.) equipped with a high load modulus. The nanoindenter applies a load via a calibrated electro-magnetic coil with a resolution of 50 nN. The displacement of the indenter was measured using a capacitive transducer with a resolution of 0.01 nm. To diﬀerentiate the values of Young’s modulus and the hardness of the microstructural constituents, a matrix of 204 (1712) indentations was made inside a representative area using a maximum load of 200 mN. The distance between the indentations was set at 5lm. The Oliver and Pharr method was used to ana-lyse the load-depth of the penetration curves and to obtain the Young’s modulus and the hardness for each location of indentation .
A similar approach was used with the indentation frac-ture toughness,Kc. A matrix of indentations (1015) was made on a representative area of the sample. A maximum load of 1 N was applied, which is large enough to induce Table 1
Projection parameters used to deposit alumina–titania coatings and Ni/ Al/Mo bond coat.
Parameter/material Bond coat Ceramic coatings
Current (A) 120 150
Voltage (V) 80 100
Working gas ﬂow, Ar (SCFH) 40 40 Projection distance (mm) 120 120 Feed powder rate (g min1) 90 80
Incident angle (°) 90 90
fracture around the imprint. The distance between the indentations was maintained at 20lm. The usual proce-dure for determining the indentation fracture toughness  cannot be applied unless a regular crack pattern is developed. Unfortunately, a regular crack pattern did not develop with the modiﬁed and conventional samples. Therefore, the indentation fracture toughness was calcu-lated by following the method described in Ref.. The coating failure is associated with pop-in events that appear as discontinuities in the loading curve. The fracture dissi-pated energy, Ufr, can be derived from the diﬀerence between the experimental curve and the hypothetical curve that is obtained in the absence of failure. After the inden-tation tests, the fractured area, Afr, around the residual imprints was measured with SEM. Finally, the indentation fracture toughness,Kc, of the coating was calculated using the following equation:
Eandvare the Young’s modulus and Poisson’s ratio of the coating, respectively. A Poisson’s ratio of 0.28 was used for all coatings.
2.2.3. Wear tests
Wear tests were carried out in a wear-testing machine (WAZAU TRM 1000) with a pin-on-disc conﬁguration under dry sliding conditions and without eliminating the formed debris. Before the test, the specimen and the count-erbody were cleaned using methanol in order to avoid the presence of humidity and other undesirable ﬁlms such as grease. The average sample roughness was always kept in the range 10 ± 3lm. Most of the procedures for the ASTM standard G99-04 were followed. However, sev-eral modiﬁcations were introduced that primarily involved the pin shape. Prismatic pins were made of the material under study (with modiﬁed and with conventional coat-ings) with a rectangular section of 2.5 mm6.3 mm. With this geometry, the nominal contact area remained constant during the tests despite the wear process. The disc was made to have the same coating as the sample and all the wear test conditions were selected according to the indus-trial application in which this material is involved. The disc rotates horizontally at a sliding speed of 0.1 m s1. A dead-weight loading system was used to perform the tests at nominal normal pressures ranging from 5 to 65 MPa. At least three tests were carried out at for each experimental condition. The coeﬃcient of friction was obtained using a torque transducer and the variation of the pin height was registered using a linear variable diﬀerential transformer with a precision of ±1lm. The pin wear rate was calcu-lated through mass measurements using a METTLER– TOLEDO balance with a resolution of 0.01 mg. The wear rate was computed using the following equation:
whereDmis the mass loss of the pin,qis the coating den-sity (3970 kg m3for both coatings),Fis the normal load andLis the sliding distance.
Finally, the worn specimens were cross-sectioned using a microcutter (Struers Accutom-5). In order to analyse the microstructural changes in the nearest zone at the pin con-tact surface, plane- and cross-sections of the worn surfaces were prepared with conventional metallographic tech-niques and observed with the help of scanning electron microscopes (Philips XL 30 and Hitachi S4400). The debris morphology and size were also examined with SEM.
The agglomerates of nanoparticles that were obtained after spray-drying were used as feeding powders for the deposition of the modiﬁed coatings. The agglomerates exhibited a spherical shape, with an average diameter of about 30lm (Fig. 1a). They were themselves formed by irregularly shaped, polygonal nanoparticles. The TEM study that was performed on the agglomerates revealed that they were composed of c-Al2O3 (Fig. 1b) and ana-tase–TiO2 (Fig. 1c). Generally, the anatase particles were the smallest, ranging from 50 to 70 nm, while thec-Al2O3 particles were approximately 200 nm.
also observed in the modiﬁed coating due to the deposition of semi-molten droplets. These microstructural features could not be found in the conventional system. The PM zones exhibited a composite microstructure, as shown in the TEM image inFig. 2d. The observed nanoparticles had an average size of 200 nm and corresponded to the alumina par-ticles that were previously identiﬁed in the feeding powders. However, the electron diﬀraction pattern indicated that a phase transition occurred during the plasma projection. The PM zones were essentially composed ofa-Al2O3, while
the main phase in the powder was c-Al2O3. Although the particles maintained their initial size, they lost the polygonal contour and displayed a smooth and round ﬁnal shape. The high temperatures reached during the projection promoted the phase transition, but the temperatures were not high enough to completely melt the particles. Thea-Al2O3 nano-particles were then embedded in a matrix that was composed of c-Al2O3nanocrystallites that were similar to those pre-sented in the FM zones. The only diﬀerence with the FM domains was that the c-Al2O3 matrix was supersaturated with Ti4+ because of the formation of a solid solution between thec-Al2O3and the TiO2. These results are in agree-ment with those obtained elsewhere[3,5,7]. Thus, the modi-ﬁed coating presents a multiphase microstructure with several levels in a hierarchical system. In fact, the microstruc-ture resembles a ceramic composite in which the matrix is mainly composed of nanocrystallites ofc-Al2O3(FM zones). The reinforcement particles (PM zones) are composed of
a-Al2O3nanoparticles embedded in ac-Al2O3matrix.
3.2. Mechanical characterization
We used depth-sensing indentation tests to determine the mechanical properties of the coatings on a local scale in order to distinguish the behaviour of each of the micro-structural constituents. These tests were performed to determine the eﬀective properties of the coatings.
3.2.1. Young’s modulus and hardness
Young’s modulus and hardness have been investigated in previous studies. A statistical analysis was performed using data from the indentation matrix that was carried out on the modiﬁed and conventional samples.Fig. 3shows the resultant histograms of the Young’s modulus and the hardness from the modiﬁed coating. Several distributions are easily identiﬁed: the ﬁrst distribution corresponds to the FM regions and the second distribution is associated with the PM particles. A third set of data were associated with the indentations that were made on pores and cracks. The experimental results yield some important observations:
– The depth-sensing indentation tests were able to dis-criminate between diﬀerent microstructural regions of the modiﬁed coating.
– The PM particles were stiﬀer and harder than the FM regions. The increased stiﬀness and hardness are likely due to the presence of a-alumina nanoparticles inside the PM particles. In addition, the FM domains were mechanically indistinguishable from the conventional coating.
– The experiments were sensitive to material defects such as pores and cracks.
To estimate the eﬀective mechanical properties of the modiﬁed coating, a simple rule of mixtures was used. The volume fraction of PM domains, VPM
f , was measured via optical microscopy and was found to be 30%. The
Fig. 1. (a) Panoramic view of the agglomerate used as feeding powder in the deposition of the modiﬁed coating. (b) TEM image of ac-alumina nanoparticle showing an electron diﬀraction pattern (EDP) with Bh1 2 3i
orientation. (c) TEM image of an anatase–TiO2particle showing an EDP
Young’s modulus and the hardness of the FM matrix and the PM reinforcement were obtained from the data pre-sented inFig. 3.Table 2outlines the main results of these tests.
3.2.2. Indentation fracture toughness
A similar statistical analysis was carried out using that fracture toughness values that were measured from the
matrix of indentations performed on the coatings. The fracture toughness histogram is presented in Fig. 4. Two distributions were exhibited by the modiﬁed coating, but a wide, single distribution was observed for the conven-tional material. The PM domains appeared to be tougher than the FM regions in the modiﬁed coating. Interestingly, the fracture toughness that was measured in the FM regions was also higher than the conventional coating. Fig. 2. Schematic representation of the hierarchical microstructure in the coatings. (a) Panoramic view of the coating system. (b) Cross-section of the modiﬁed coating showing a partially melted zone embedded in a fully melted region. (c) Cross-section of the conventional coating showing the typical APS coating’s splat morphology. (d) TEM image showing the morphology and composition of nanoparticles inside the partially melted zone from the modiﬁed coating. An EDP corresponding to ana-Al2O3nanoparticle with a Bh1 1 1iorientation and an EDP corresponding to the surrounding matrix are also
Rose suggested a model to estimate the eﬀective fracture toughness for a composite made of a brittle matrix that is reinforced by well-bonded particles . This description generally applies to the material studied here. In terms of the modiﬁed coating parameters, the model can be writ-ten as:
KMOD c ¼K
KPM c KFM
whereRis the particle radius,Lis the centre-to-centre dis-tance of the particles.KMOD
c ,K PM c andK
c are the eﬀective fracture toughness of the modiﬁed coating, the fracture toughness of the PM domain and the fracture toughness for the FM region, respectively. Expression (3) is a rule Fig. 3. Statistical distribution for the mechanical properties of the
modiﬁed coating obtained from depth-sensing indentation analysis. (a) Young’s modulus. (b) Hardness.
Mechanical properties of the coatings measured by means of depth-sensing indentation.
Modiﬁed coating Conventional coating
PM domain FM domain Eﬀective property
Young’s modulus,E(GPa) 300 ± 16 269 ± 18 278 ± 17a 265 ± 15
Hardness (GPa) 14.0 ± 0.9 9.7 ± 1.1 11 ± 1.0a 9.6 ± 0.7
Fracture toughness (MPa m1/2) 5.4 ± 0.7 3.0 ± 0.8 4.8 ± 0.8b 2.2 ± 0.8
a Using a simple rule of mixtures. b Using Eq.(3).
of mixtures that was applied to the speciﬁc fracture energy,
Gc. The propagation of a crack in a brittle matrix rein-forced by well-bonded particles was further investigated by Bower and Ortiz , who used a numerical analysis to demonstrate that the Rose model ﬁt well with the exper-imental data ifR/Lwas in a range from 0 to 0.3. The ratio
R/L in the modiﬁed material remained approximately in this range. Accordingly, Eq. (3) was applied in order to estimate the eﬀective fracture toughness of the modiﬁed coating using the data fromFig. 4. A summary of the cal-culated results is compiled inTable 2.
3.3. Tribological behaviour
3.3.1. Wear rate and friction coeﬃcient
Fig. 5a shows the wear rate of the coatings vs. a nominal normal pressure. The modiﬁed coating exhibited lower wear rates than the conventional coating for all of the experimental conditions. When the normal pressure was low (<15 MPa), the diﬀerences between the dissimilar coat-ings reached a factor close to 4. Both of the materials dis-played evidence of a transition between the mild and severe wear regimes (marked with arrows inFig. 5a), as detected by abrupt increases in the wear rate and the friction coeﬃ-cient values (Fig. 5b). This transition was associated with wear rate changes of up to two orders of magnitude. The critical normal pressure at which the transition was pro-moted was higher in the modiﬁed coating and highlights the superior protection oﬀered by this material relative to the conventional one. The values of the critical normal pressures were 20 and 40 MPa for the conventional and modiﬁed coatings, respectively.
The friction coeﬃcient vs. the nominal pressure data is presented inFig. 5b. A transition between mild and severe wear was also observed, but the critical pressure was higher for the modiﬁed coating than for the conventional one. Although the transition was delayed in the modiﬁed coat-ing, the values corresponding to mild wear (l0.5) and severe wear (l0.85) were similar in both coatings.
3.3.2. Wear mechanisms
The transition detected in the wear rate and the friction coeﬃcient suggests that the wear mechanism is dependent upon the nominal normal pressure. The worn surfaces of the conventional and the modiﬁed coatings that were tested at low normal pressures (5 MPa) are presented in Fig. 6. Brittle crack propagation through the splat boundaries seemed to be the operative wear mechanism in the mild wear regime. The crack propagation along the splat bound-aries was especially evident in the conventional coating (Fig. 6a). However, in the modiﬁed coating, the PM zones were capable of deﬂecting cracks that obstructed its prop-agation (Fig. 6b). The role played by the PM zones is trib-ologically signiﬁcant and could also justify the increase in the coating fracture toughness shown in Table 2.
In agreement with Williams , “Each of the various processes by which material can be lost from a surface in
the modiﬁed coating is shown inFig. 7b. The crack deﬂects around the PM particle and increases the wear resistance of the material.
Histograms that show the size distribution of the debris particles obtained in the mild wear regime are presented in Fig. 8. Although a wide distribution was observed, an average value could be determined for each material. The average debris size for the conventional coating was approximately 30lm. In the modiﬁed material, the average debris size was closer to 42lm. The debris size values were correlated with microstructural features (seeFig. 2). In the conventional coating, the debris size was similar to the splat size. In the modiﬁed coating, it was comparable to the space between PM zones if a regular distribution was assumed.
When tests were implemented in the severe wear regime, brittle crack propagation remained the primary wear mech-anism (Fig. 9); however, the crack patterns were diﬀerent. Large transverse cracks crossed the splat borders in both types of coating (Fig. 9a and b). The FM/PM interfaces were also fractured in the modiﬁed coating (Fig. 9c). Cracks can easily reach the interface between the ceramic coating and the metallic bond coat, introduce damage to the material in the form of complete spallation and pro-duce an abrupt increase in the wear rates by several orders
of magnitude. The friction coeﬃcient also exhibited a sub-stantial increase in this regime, which may be explained by the higher roughness of the worn surfaces.
The delay in the transition from mild to severe wear in the modiﬁed material is assumed to be due to the eﬀect of the PM particles on the crack propagation. The PM par-ticles must postpone the activation of the trans-splat mech-anism at higher nominal pressures and, when the contact severity is high enough to allow the crack to penetrate into the PM zone, a new deﬂection mechanism at a lower scale (200 nm) is triggered around the a-Al2O3 nanoparticles (Fig. 9c). Again, this process is a consequence of the hier-archical microstructure that is formed during the thermal deposition.
The debris morphology can also be related to the wear mechanism in the severe regime. In Fig. 10a, an example of a debris particle that was removed from the conven-tional coating is shown. The particles are larger than those obtained from low normal pressure tests. Brittle fracture features are visible. A detail of the conventional debris par-ticle is shown inFig. 10b, indicating the presence of broken splats that reveal a trans-splat mechanism. Fig. 11 shows debris particles that were obtained from the modiﬁed coating that had cracks crossing the FM zones (splats) and the PM particles. The deﬂection mechanism around
Fig. 6. SEM images showing plan views of the worn surfaces obtained from tests performed at mild wear conditions (5 MPa). (a) Conventional. (b) Modiﬁed.
thea-Al2O3nanoparticles is also shown (Fig. 11b and c). The presence of these 200 nm particles in the PM regions not only improves its mechanical properties, but also acti-vates wear mechanisms that do not exist in the FM zones or in the conventional material.
In Fig. 12, histograms of the debris size distribution under severe wear conditions are shown. The mean values are larger than those obtained in the mild wear regime. The mean size is larger for the modiﬁed material than for the conventional one.
The wear tests revealed that brittle crack propagation is the primary wear mechanism observed, meaning that frac-ture toughness should be the key material property. In addition, both the modiﬁed and the conventional coatings displayed a transition between the mild and the severe wear regimes. This transition was detected by an abrupt increase
of several orders of magnitude in the wear rate, an augmen-tation in the friction coeﬃcient, a change in the crack path propagation and a variation of the debris size. In the mild wear regime, the cracks grow along the splat borders. In the severe wear regime, cracks transversely propagate through the ceramic layer and sometimes cross the splats and PM zones.
The analysis of the factors that aﬀect the wear behaviour was complex. The wear resistance is not a material property, Fig. 8. Histograms showing the debris size distribution at mild wear
conditions. (a) Conventional. (b) Modiﬁed.
but it depends upon mechanical performance and operating parameters such as load, sliding velocity and temperature.
In this study, the material wear resistance was investi-gated by making energetic considerations. The ﬁnal aim of this work was to build a wear map that uses dimension-less parameters (including material properties and working conditions) and explains why the modiﬁed coating pre-sented better wear behaviour than the conventional one.
To describe the material wear behaviour, the dimension-less wear coeﬃcient,kH(kis the wear rate andHthe mate-rial hardness), can be written as a function,U, of the ratio between the input energy, I, and the energy that is dissi-pated by the material during the wear process,D:
kH ¼U I
The large number of variables aﬀecting the wear behav-iour makes it diﬃcult to determine the right form forIand
D. There are several ways to establish these expressions but, among them, dimensional analysis was adequate. This methodology is based on the Buckingham theorem . Every physical magnitude (i.e. the wear rate) can be corre-lated with a group of dimensionless ratios that comprise the physical variables that are responsible for the phenome-non (the wear, in the case of this study). The main diﬃculty of
this method lies in the fact that the parameters that inﬂuence the problem must be known a priori.
The primary wear mechanism was brittle crack propaga-tion. Consequently, the fracture toughness,Kc, hardness,H, and Young’s modulus, E, were the relevant mechanical properties to explain the observed results. Because a fraction of the input energy is dissipated through frictional heating, properties like the speciﬁc heat,cp, and the thermal conduc-tivity,kT, must be included in the analysis. Together with the density,q, the thermal diﬀusivity,d, comprises all of these parameters. On the other hand, the operation conditions such as normal nominal pressure,p, and the sliding velocity,
v, should be considered in the analysis. Furthermore, several parameters that account for the properties of the particular contact must be added. The friction coeﬃcient, l, and the equivalent contact radius,req(the square root of the nominal contact area divided by p), can be used for this purpose. Finally, a characteristic length must be included in order to satisfy the dimensional analysis requirements. The average debris size,l*, was chosen because this parameter incorpo-rates the values that represent each material and wear regime.
Using the Buckingham theorem , it is possible to write the wear coeﬃcient, kH, as a potential function that depends upon the rest of the variables that are grouped
Fig. 10. SEM images showing the debris obtained from conventional coatings at severe wear conditions (65 MPa). (a) Panoramic view. (b) Detail from (a).
Broken splats Splat (FM
into a series of dimensionless ratios. The solution leads to the next expression:
kH ¼C ln1 P
The choice of the ni exponents is arbitrary. Two approaches exist to establish the value for these exponents. The ﬁrst approach consists of setting their values through the best ﬁt of the experimental data. The second approach selects these exponents from a physical point of view. This second option allows for interpretation of the involved physical phenomenon because the relevance on the wear rate of each variable is taken into account. Proceeding in this way, the following expression was obtained:
kH ¼C lPvreqE 2l0
¼C lP H
¼C lP v G
whereGis the energy-release rate of the material. This rate was introduced using the plane stress relationship between
Gand fracture toughnessKc(16):
Gis the dimensionless form ofGdeﬁned asG¼ G El. There
is no reason to assume plane stress or plane strain condi-tions but, if the Poisson’s ratio of these materials is taken into account, the diﬀerences are lower than 10%. The load and sliding velocity can be written in dimensionless form as P¼P
H andv¼ vreq
d , respectively.
The ﬁnal form of Eq.(6)is similar to Eq.(4). The wear coeﬃcient, kH, depends on a parameter that relates a dimensionless form of the input energy of the tribosystem,
lP v, and the dimensionless form of the energy that is con-sumed during crack propagation through the material,G. In this particular case, the primary wear mechanism is the brittle propagation of cracks, and it follows that the en-ergy consumption is adequately expressed viaG.
The termðlP v
GÞin Eq.(6) can be interpreted as a contact
severity parameter by adopting the terminology previously used in the literature. Under the same operation condi-tions (normal load, sliding velocity), a material with a minor contact severity should exhibit a lower wear rate as a result of its better mechanical behaviour.
One question remains for consideration. Similar contact severities should lead to similar wear coeﬃcients if the phe-nomenon is controlled by the same wear mechanism. In Fig. 13, the wear coeﬃcient,kH, is plotted for both mate-rials vs. the dimensionless parameterðlGP vÞ. The experimen-tal data that correspond to both materials are described by the same curve, conﬁrming the previous argument. In addi-tion, the wear data that correspond to the modiﬁed coating are shifted to the low severity contact values as a result of its better mechanical properties (seeTable 2), while those Fig. 12. Histograms showing the debris size distribution at severe wear
conditions. (a) Conventional. (b) Modiﬁed.
of the conventional coating are clearly displaced to higher contact severities. The modiﬁed coating microstructure has better eﬀective mechanical properties (E,HandKc), which are incorporated into the global wear parameterðlP v
multiphase character of the modiﬁed coating leads to lower values of this dimensionless factor.
The values of the parameters C and n in Eq. (6) are aﬀected by all the magnitudes that are not considered in the analysis: contact geometry, surface roughness, type of movement, etc. Nevertheless, the experimental procedure (Section2) showed that all of these testing conditions were the same for both coatings. The uniformity of the testing conditions enables the comparison shown inFig. 13.
The main practical obstacle in the analysis presented here is that the size of the wear debris is not known before the test is performed, and this obstacle limits the prediction capabil-ity. This problem can be solved in those cases where the deb-ris size can be related to any microstructural feature through a priori determination. This study seems to show a relation-ship between the debris and the splat sizes in the mild wear of the conventional coating. A similar result can be found for the modiﬁed coating mild wear because the mean debris size is correlated with the interparticle spacing between PM zones. Under severe wear conditions, no link between the debris size and microstructural features can be conﬁrmed.
Mechanical and tribological characterization has been carried out on Al2O3–13% TiO2conventional and modiﬁed coatings that were deposited by atmospheric plasma spray. The following conclusions were drawn:
A statistical analysis of the Young’s modulus, hardness and fracture toughness data were performed. Independent of the mechanical properties, the modiﬁed coating is assumed to behave as a composite material. The properties of each constituent (PM and FM domains) were deter-mined by depth-sensing indentation, and the eﬀective prop-erties of the coatings were obtained via a rule of mixtures. An energetic approach, developed through dimensional analysis, has been used to explain wear data. The wear rate, put in terms of the wear coeﬃcient,kH, has been expressed as a function of a dimensionless parameter that comprises a form of the input energy to the tribosystem and a form of the energy dissipated by the material during the wear pro-cess. The input energy can be expressed as the product of the friction coeﬃcient, the normalized normal pressure and the normalized sliding velocity. The key to this meth-odology is the fact that the dissipated energy depends upon the operation wear mechanism. When the main wear mech-anism is brittle crack propagation, the dissipated energy can be written as a dimensionless function of the energy-release rate,G. If the wear coeﬃcient is represented in rela-tion to the dimensionless contact severity parameter,ðlP v
the wear data that correspond to both coatings can be described by the same function.
The multiphase character of the modiﬁed coating was described through its eﬀective Young’s modulus, hardness and fracture toughness. We propose that the global wear behaviour of a material is governed by its global or eﬀective properties. The materials studied in this work, conventional and modiﬁed, have the same composition but diﬀerent microstructural features; consequently, they have diﬀerent eﬀective properties. Their wear behaviour is clearly diﬀer-ent, but it can be described by the same equation because dimensionless parameters were used and the same wear mechanism was observed in both cases. The diﬀerent behav-iour was determined through the eﬀective mechanical prop-erties of each coating.
The authors are indebted to Comunidad de Madrid for its ﬁnancial support through the ESTRUMAT program. Thanks are also extended to Dr. A. Salazar for her help during the manuscript revision.
 Ananthapadmanabhan PV, Thiyagarajan TK, Satpute RU, Venkatr-amani N, Ramachandran K. Surf Coat Technol 2003;168:231–40.  Ramachandran K, Selvarajan V, Ananthapadmanabhan PV,
Sreeku-mar KP. Thin Solid Films 1998;315:144–52.
 Erickson LC, Hawthorne HM, Troczynski T. Wear 2001;250:569–75.  Pantelis DI, Psyllaki P, Alexopoulos N. Wear 2000;237:197–204.  Gessasma S, Bounazef M, Nardin P, Sahraoui T. Ceram Int
 Normand B, Fervel V, Coddet C, Nikitine V. Surf Coat Technol 2000;123:278–87.
 Shaw LL, Goberman D, Ren R, Gell M, Jiang S, Wang Y, et al. Surf Coat Technol 2000;130:1–8.
 Wang Y, Jiang S, Wang M, Wang S, Xiao TD, Strutt PR. Wear 2000;237:176–85.
 Gell M, Jordan EH, Sohn YH, Shaw L, Xiao TD. Surf Coat Technol 2001;146–147:48–54.
 Jordan EH, Gell M, Sohn YH, Goberman D, Shaw L, Jiang S, et al. Mater Sci Eng 2001;A301:80–9.
 Goberman D, Sohn YH, Shaw L, Jordan E, Gell. Acta Mater 2002;50:1141–52.
 Liu Y, Fischer ET, Dent A. Surf Coat Technol 2003;167:68–76.  Bansal P, Padture NP, Vasiliev A. Acta Mater 2003;51:2959–70.  Lin X, Zeng Y, Lee SW, Ding C. J Eur Ceram Soc 2004;24:627–34.  Cao XQ, Vassen R, Schwartz S, Jungen W, Tietz F, Sto¨ever D. J Eur
Ceram Soc 2000;20:2433–9.
 Rodriguez J, Rico A, Otero E, Rainforth WM. Acta Mater 2009;57:3148–56.
 Rico A, Rodriguez J, Otero E, Zeng P, Rainforth WM. Wear 2009;267:1191–7.
 Rico A. PhD dissertation, Universidad Rey Juan Carlos, Madrid; 2009.
 Adachi K, Kato K, Chen N. Wear 1997;203–204:291–301.  Hsu SM, Wang YS, Munro RG. Wear 1989;134:1–11.
 Kato K. In: Proceedings of the international tribology conference; 1995. p. 421–6.
 Hokkirigawa K, Kato K. In: Proceedings of the 33rd JSLE conference; 1989. p. 9–12.
 Dong X, Jahanmir S, Hsu SM. J Am Ceram Soc 1991;74 5:1036–44.  Dong X, Jahanmir S. Wear 1993;165:169–80.
 Akazawa M. In: Proceedings of the international congress on tribology—5th Eurotrib’89; 1989. p. 126–31.
 Hokkirigawa K, Kato K, Araya S. In: Proceedings of the Japan international tribology conference; 1990. p. 1425–30.
 Xu J, Kato K. In: Proceedings of the international sympo-sium on microsystems, intelligent materials and robots; 1995. p. 122–5.
 Chen N, Adachi K, Kato K. Trans JSME C 61 1995;584: 1605–12.
 Lim SC, Ashby MF. Acta Metall 1987;35(1):1–24.  Antoniou R, Subrananian C. Scripta Metall 1989;22:80–3.
 Childs T.H. In: Proceedings of the institution of mechanical engineers, vol. 20(2); 1988. p. 379–95 (C6).
 Briscoe BJ, Evans PD. In: Proceedings of the wear of materials; 1989. p. 449–57.
 Kato K, Hokkirigawa K. In: Proceedings of the international congress of Tribology—Eurotrib’85; 1985. p. 1–5.
 Hsu SM, Shen M. Wear 2004;256:867–78.
 Oliver WC, Pharr GM. J Mater Res 1992;7:1564–83.
 Anstis GR, Chantikul P, Lawn BR, Marshall DB. J Am Ceram Soc 1981;64:533–8.
 Li X, Diao D, Bushan B. Acta Mater 1997;44:4453–61.
 ASTM G99-04. Standard test method for wear testing with a pin on disk apparatus; 1999.
 Rose LRF. Mech Mater 1987;6:11.
 Bower AF, Ortiz M. J Mech Phys Solids 1991;39:815.  Williams JA. Tribol Int 2005;28:863–70.